- 81 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about ' VIII. Kinematical Theory of Diffraction' - anakin

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

VIII. Kinematical Theory of Diffraction

8-1. Total Scattering Amplitude

The path difference

between beams

scattered from the

volume element

apart is

The amplitude of the wave scattered from a

volume element is proportional to the local

electron concentration ! Why?

Define

: periodic function in a crystal

A periodic function can be expanded by

Fourier series!

Any criteria to expand it?

Physical properties function of a crystal

Crystal translation vector

Periodic function Exponential Fourier Series

u, v, w: integer

Translation vectors of the original crystal lattice

for all

h, k, l: integer

If

Vectors of the reciprocal lattice

The total scattering amplitude F

structure factor

For a unit cell, total electron concentration at

due to all atoms in the unit cell

The scattering amplitude is then expressed as

8-2. Atomic form factor calculation

The meaning of form factor is equivalent

to the total charge of an atom, which can be

obtained by a direct calculation.

With the integral extended over the electron

concentration associated with a single

atom, set the origin at the atom

Spherical integration dV = dr(rd)(rsind)

r: 0 -

: 0 -

: 0 - 2

http://pleasemakeanote.blogspot.tw/2010/02/9-derivation-of-continuity-equation-in.html

depends on G

When

total number of

electron in an atom

Tabulated

Function of element and diffracted angle

Si, 400 diffraction peak, with Cu K (0.1542 nm)

0

0.1

0.2

0.3

0.4

0.5

0.6

14.0

12.16

9.67

8.22

7.20

6.24

5.31

or

8-3. Structure Factor Calculation

(a) Primitive cell

1 atoms/unit cell;

000 and 100, 010, 001, 110, 101, 011, 111:

equipointsof rank 1; Choose any one will have

the same result!

for all hkl

2 atoms/unit cell;

000 and 100, 010, 001, 110, 101, 011, 111:

equipointsof rank 1;

½ ½ 0, ½ ½ 1 : equipoints of rank 1;

Two points chosen: 000 and ½ ½ 0.

If h , k is unmixed or h + k is even

If h ,k is mixed or h +k is odd

The meaning of the reflection condition

(reflection rule)

Suppose that we have a square lattice

(a) Primitive unit cell：one atom at [00]

The reflection conditions remove the lattice

points [odd, 0] in the reciprocal lattice.

Therefore, the meaning of the reflection rule is

to remove the additional lattice points due to the

selection of unit cell.

After the substraction, the reciprocal lattice

structures derived from both cases (primitive

unit cell and unit cell) become the same.

2 atoms/unit cell;

000 and 100, 010, 001, 110, 101, 011, 111:

equipointsof rank 1;

½ ½ ½: equipoints of rank 1;

Two points to choose: 000 and ½ ½ ½.

If h + k + l is even

If h + k + l is odd

4 atoms/unit cell;

000 and 100, 010, 001, 110, 101, 011, 111:

equipointsof rank 1;

½ ½ 0, ½ 0 ½, 0 ½ ½, ½ ½ 1, ½ 1 ½, 1 ½ ½: :

equipoints of rank 3;

Four points chosen: 000, ½½0, ½0½, 0½½

If h, k, l mixed

(e) close-packed hexagonal cell

2 atoms/unit cell

8 corner atoms: equipointsof rank 1;

2/3 1/3 1/2: equipoints of rank 1;

Choose 000, 2/3 1/3 1/2. (Miller Indices)

(f) ZnS: four Zinc and four sulfur atoms per

unit cell (8 atoms/unit cell)

000 and 100, 010, 001, 110, 101, 011, 111:

equipoints of rank 1; (S atom)

½½0, ½0½, 0½½, ½½1, ½1½, 1½½:

equipoints of rank 3; (S atom)

¼¼¼, ¾¾¼, ¾¼¾, ¼¾¾:equipoints of rank 4; (Zn)

Eight atoms chosen: 000, ½½0, ½0½,

0½½ (the same as FCC), (Say S atom)

¼¼¼, ¾¾¼, ¾¼¾, ¼¾¾ (Say Zn atom)!

h, k, l: unmixed

when h, k, l are all odd

when h, k, l are all even and h + k + l = 4n

when h, k, l are all even and h + k + l4n

Therefore, for a finite crystal, the diffracted

intensity is finite based on the condition below.

I 0 if

Example: for a very thin sample

Ewald sphere construction

When

diffraction occurs due

to “shape effect”.

Download Presentation

Connecting to Server..